Cast iron is made when pig iron is re-
melted in small cupola furnaces (similar
to the blast furnace in design and
operation) and poured into molds to
make castings. Cast Iron is generally
defined as an alloy of Iron with greater
than 2% Carbon, and usually with more
than 0.1% Silicon.
Exception: Silicon and other alloying
elements may considerably change the
maximum solubility of Carbon in
Austenite. Thus certain alloys can
solidify with a eutectic structure having
less than 2% Carbon.
Cast iron has its earliest origins in China between 700
and 800 B.C.
Until this period ancient furnaces could not reach
sufficiently high temperatures.
The use of this newly discovered form of iron varied from
simple tools to a complex chain suspension bridge
erected approximately 56 A.D.
Cast iron was not produced in mass quantity until
fourteenth centaury A.D.
White Iron: large amount of carbide
phases in the form of flakes,
surrounded by a matrix of either
Pearlite or Martensite. The result of
metastable solidification. Has a
white crystalline fracture surface
because fracture occurs along the
iron carbide plates. Considerable
strength, insignificant ductility.
Gray Iron: Graphite flakes
surrounded by a matrix of either
Pearlite or α−Ferrite. Exhibits gray
fracture surface due to fracture
occurring along Graphite plates.
The product of a stable
strength, insignificant ductility.
Microstructure of White Cast Iron
Microstructure of Gray Cast Iron
Ductile (Nodular) Iron:
Graphite nodules surrounded
by a matrix of either α−Ferrite,
Bainite, or Austenite. Exhibits
substantial ductility in its as
Malleable Iron: cast as White
Iron, then malleabilized, or
heat treated, to impart ductility.
Consists of tempered
Graphite in an α−Ferrite or
Microstructure of Ductile Iron
Microstructure of Malleable Iron
Graphite structure is a factored
crystal bounded by low index planes.
Growth occurs along (ı0ī0) & (000ı)
planes (direction A & C). Unstable
growth occurs along direction A,
giving the Graphite microstructure
rough, poorly defined, edges in
When grown from the solidification
of liquid Iron Carbon alloys, Graphite
takes on a layer structure. Among
each layer covalent chemical bonds
with strengths between (4.19E5 -
5E5)J/mol exist. Between layers
weaker bonds exist on the order of
(4.19E3 - 8.37E3)J/mol.
The structure of the Graphite
depends on the chemical
composition, the ratio of temperature
gradient to growth rate, and the
cooling rate. Such structures are:
Flake or Plate Graphite (a)
Coral Graphite (c)
Spheroidal Graphite (d)
A wide variety of
compounds and certain
metals have been claimed
to serve as either
inoculants or nuclei for
Flake Graphite growth.
(Silicon dioxide, silicates,
sulfides, boron nitride,
potassium, calcium, ect...)
Two methods of growth.
The nucleation of Flake
Graphite Iron occurs
mainly on silicon dioxide
Salt like carbides
containing the ion Carbon
are used as inoculants.
Such carbides include
NaHC2 & KHC2 from
Group I, CaC2, SrC2,
BaC2 from group II, and
YC2 & LaC2 from group III.
White Cast Irons contain
Chromium to prevent formation of
Graphite upon solidification and to
ensure stability of the carbide
phase. Usually, Nickel,
Molybdenum, and/or Copper are
alloyed to prevent to the formation
of Pearlite when a matrix of
Martensite is desired.
Fall into three major groups:
Nickel Chromium White Irons:
containing 3-5%Ni, 1-4%Cr.
Identified by the name Ni-Hard 1-4
irons (high chromium irons): 11-
23%Cr, 3%Mo, and sometimes
additionally alloyed w/ Ni or Cu.
25-28%Cr White Irons:
contain other alloying additions of
Molybdenum and/or Nickel up to
Gray Cast Irons contain silicon, in addition to carbon, as a
primary alloy. Amounts of manganese are also added to yield
the desired microstructure. Generally the graphite exists in the
form of flakes, which are surrounded by an a-ferrite or Pearlite
matrix. Most Gray Irons are hypoeutectic, meaning they have
carbon equivalence (C.E.) of less than 4.3.
Gray cast irons are comparatively weak and brittle in tension due
to its microstructure; the graphite flakes have tips which serve as
points of stress concentration. Strength and ductility are much
higher under compression loads.
As a liquid, Ductile Iron has a high fluidity, excellent
castability, but high surface tension. Thus, sands and
molding equipment must provide molds of high density and
good heat transfer.
Solidification of Ductile Cast Iron usually occurs with no
appreciable shrinkage or expansion due to the expansion
of the graphite nodules counteracting the shrinkage of the
Iron matrix. Thus, risers (reservoirs in mold that feed
molten metal into the cavity to compensate for a decrease
in volume) are rarely used.
Require less compensation for shrinkage. (Designers
compensate for shrinkage by casting molds that are larger
Most Ductile Irons used as cast. Heat treating (except for
austempering) decreases fatigue properties. Example:
Holding at the subcritical temperature (705˚C) for ≈ 4 hours
improves fatigue resistance. While heating above 790˚C
followed by either an air or oil quench, or ferritizing by
heating to 900˚C and slow cooling reduces fatigue strength
and fatigue resistance in most warm environments.
Austempered Ductile Iron has been considered for most
applications in recent years due to its combination of
desirable properties. A matrix of Bainitic Ferrite and
stabilized Austenite with Graphite nodules embedded.
Applications include: Gears, wear resistant parts, High-
fatigue strength applications, High-impact strength
applications, automotive crankshafts, Chain sprockets,
Refrigeration compressor crankshafts, Universal joints,
Chain links, and Dolly wheels.
Used for a variety of applications, specifically those requiring strength and
toughness along with good machinability and low cost. Casting, rather than
mechanical fabrication (such as welding), allows the user to optimize the
properties of the material, combine several castings into a desired configuration,
and realize the economic advantages inherent in casting.
Microstructure is consistent; machinability is low due to casting forming the
desired shape; porosity is predictable and remains in the thermal center.
Ductile Iron can be austempered to high tensile strength, fatigue strength,
toughness, and wear resistance. Lower density
Ductile Iron seems to work in applications where theories suggest it should
Ductile Iron shipments exceeded 4 million in 95.
Cast Iron pipe make up to 44% of those shipments.
29% used for automobiles and light trucks (economic advantages and high
Other important applications are: Papermaking machinery; Farm equipment;
Construction machinery and equipment; Power transmission components
(gears); Oilfield equipment.
Type of Iron with Graphite in the form of
irregularly shaped nodules.
Produced by first casting the Iron as a White
Iron, then heat treating to transform the
Carbide into Graphite.
Categorized into 3 categories: Ferritic,
Pearlitic, and Martensitic Malleable Cast Iron.
Two types of Ferritic: Blackheart (top) and
Whiteheart (not produced in US)
Posses’ considerable ductility and
toughness due to the combination of nodular
graphite and low carbon matrix. Often a choice
between Malleable and Ductile Iron for some
applications, decided by economic constraints.
Solidification of white Iron throughout a
section is essential in producing Malleable Iron,
thus, applications of large cross section are
usually Ductile Irons.
Usually capable in section thickness
between 1.5-100mm (1/16 4 in) and 30g (1oz) -
180 kg (400lb)
Preferred in the following applications: This
section casting; parts that are to be pieced,
coined, or cold worked; parts requiring max
machinability; parts that must retain good
impact resistance at low temp; parts requiring
Essential parts in trains,
frames, suspensions, and
differential cases, bearing
caps, steering-gear housings,
spring hangers, universal-joint
yokes, automatic transmission
parts, rocker arms, disc brake
calipers, wheel hubs, ect...
a) Driveline yokes, b)
Connecting rods, c) Diesel
pumps, d) Steering-gear
Possible to identify and classify a sample of
unknown cast iron.
Identification can be accomplished through the
use of many known mechanical, chemical and
structural properties of the cast iron alloys.
As part of our research, we attempted to
examine and identify separate cast iron samples
of unknown composition.
We obtained two samples of
what was initially perceived to
be cast iron. The first being a
cooking pot, and the second a
90° pipe fitting.
Both samples were cut,
mounted and polished in a
bakelite round, for
Followed by a Rockwell
hardness test of each
The microstructure analysis was accomplished
after polishing and etching (utilizing a 3% nitric
acid solution in ethanol) to reveal the grains.
Initially it was believed that both samples were
cast irons, and although the 90° pipe fitting
appears to be cast iron, the microstructure of the
pot handle yielded a different conclusion.
The two micrographs are shown above, the 90° pipe fitting on the
left, and the cooking pot handle on the right.
The Rockwell hardness was also measured for both samples,
yielding a hardness of 157 HRB for the fitting, and 120 HRB for the
Upon analysis of the microstructures, it became
apparent that the cooking pot does not conform to
any common form of cast iron.
Although the handle fractured in a manner very
similar to that of cast iron, the microstructure shows
little resemblance to those of cast iron.
Although further analysis would be required, one
possibility is a cast steel material. This would account
for the similarity of its fracture to that of cast iron.
The 90° fitting shows indications of a
dark graphite surrounded by lighter
colored matrix. The graphite appears
to be in the form of dark rosettes,
while the matrix is a lighter color.
Upon comparison to the known
structure of different types of cast
irons, it can be seen that the
microstructure of malleable iron most
closely matches our sample.
To the right is a side-by-side
comparison, with our sample on the
top, and a known Malleable
microstructure on the bottom.
Pipe Sample (150X mag)
Malleable Iron (150X mag)
Cast Iron and historical significance
◦ Used throughout history since its discovery, stepping stone to the
development of modern technology (First Steam Engine)
Types of Cast Irons and microstructure
◦ Grays, Whites, Ductile, Malleable
◦ Automotive, Industrial, Household, Aeronautical, & Construction
Sample Analysis and Comparison for identification and Classification
◦ Capability to analyze and compare microstructures to determine Cast Iron
Type. And Hardness measurements to identify heat treatment,
1. C.F. Walton, Gray and Ductile Iron Castings Handbook, Iron
Founder’s Society, 1971, p 193
2. C.F. Walton and T.J. Opar, Iron Castings Handbook, Iron Casting
Society, 1981, p 235 & p 297-321
3. “Chrome-Moly White Cast Irons,” Publication M – 630, AMAX, Inc.,
4. Davis, J.R., Cast Irons, ASM International, Materials Park, OH,
5. G. Lambert, Ed., Typical Microstructures of Cast Metals, 2nd
The Institute of British Foundrymen, 1996, p 47
6. H.T. Angus, Physical and Engineering Properties of Cast Iron,
BCIRA, 1960, p 21